Yang Alternatives to hard chromium plating on piston rods Degree Project of 30 credit points
As a main part of hydraulic cylinder, the piston rod is used in tough surrounding and corrosive condition; consequently a high quality protecting layer is essential. Currently EHC, electroplating hard chromium (hard chrome) is a widespread method for piston rod due to powerful performance and low cost. Unfortunately the plating process contains hexavalent chromium (Cr) which is toxic and carcinogenic; perhaps it will be prohibited in the nearing future. Therefore it is crucial to seeking alternatives to hard chrome for piston rod manufacturer. Through extensive searching for alternatives to hard chrome, the competitors like HVOF, electroplating tungsten plating and stainless steel linear were studied in the present work. Since microhardness and corrosion resistance are top priorities, after comparison perhaps Cr3C2-NiCr20% HVOF is the most promising technique. Distinct pretreatments Cr3C2-NiCr coatings were compared with hard chrome in pendulum impact test, hardness test and acetic acid salt spray (AASS) test. The results indicate that hard chrome show higher toughness more than 40% compare with HVOF, the microhardness of HVOF is higher than hard chrome, mean value 1784 Vs. 1244 HV and both coatings have excellent bonding strength. After 40 hours in AASS test, the hard chrome was rated No. 10, however the HVOF just No. 6.
Tribological Requirements of Thermally Sprayed Coatings for Wear Resistant Applications
During the last decades, improved understanding of tribological behavior of different material combinations led also to an intensified development of thermal spray applications. In the field of e.g. hard chromium replacement by thermal spraying, significant amount of work has been done and published world wide, however, the authors manly focussed on only one tribological aspect like friction, abrasion, erosion, cavitation or corrosion, respectively. In real applications, often more than one of those factors influence the successful use of these coatings. Besides the bulk properties of the materials, the coating micro structure, which is strongly spray system dependent, needs to be considered and investigated. Higher functionality and reliability than conventional competitive coatings still has to be proved at laboratory scale and under field conditions for thermally sprayed coatings. This paper describes the state of the art of thermally sprayed coatings as alternatives for other coatings. Published literature data and a wide range of own tribological investigations and field tests, reveals the potential for other applications.
Hygroscopic Expansion of some Casting Investments
CREDIT is generally given to Taggart1 for introducing the cast gold inlay to the dental profession. Although he realized that gold shrinks when cooled from molten state to solid state of room temperature, the investment available to him did not supply sufficient compensation. In 1910, Van Horn2 published a paper dealing with a method by which he obtained the compensation by means of wax expansion. The next major research in connection with this problem was the work of Coleman3 at the National Bureau of Standards. He determined the gold shrinkage to be 1.25 per cent and presented a casting technic with compensation values of quantitative nature. The total compensation for the gold shrinkage was obtained by the combination of the setting and thermal expansion of the mold. This procedure is the general practice followed at the present time for compensation. There are some disadvantages to this method. Skinner has indicated the difficulty of obtaining smooth castings and the improper compensation for the casting shrinkage.4 It has been found by Hollenback5 and Scheu6a that castings made at a high temperature are rougher than those made at a low temperature (450° C.), depending upon the great difference in thermal expansion between plaster of Paris and silica, which causes a poor union of the fine particles. This may also result in friability and there may be some warpage due to the differential expansion. A method which provides sufficient compensation at a low mold temperature is the hygroscopic casting technic.b Wilson7 showed that certain plasters expand as much as 0.0044 inch to the inch by taking up moisture from the air. With this information at hand, Scheula, b tested some commercial investment to determine what results the addition of moisture would have. He found6b: (1) All of the casting investments that were tested expanded. (2) The thicker the mix, the greater the expansion. (3) A mix with hot water expanded more than one with cold water. (4) The time at which the mix is placed in the water is of great importance. It was found that if the mix is placed in the water early, it would not expand so much as when placed in a little later. It was also found that if the mix was placed in the water after a certain time, it could not expand to the maximal amount. (5) The temperature of the water in which the mix is placed is important, for two reasons; (a) the temperature of the water controls slightly the expansion of the investment, and (b) water at a temperature of 1000 F. slightly softens the wax pattern so that the fine margins are not marred while expansion is taking place. The mix should remain in the water at least 20 minutes to obtain the full expansion, after which time no further expansion is obtained.